Plane Strain Test for Metal Sheet Characterization


 Terence Stevenson
 1 years ago
 Views:
Transcription
1 Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue du Président Wilson 62, Cachan Cedex, France 3 Department of ArGEnCO, University of Liège, Chemin des Chevreuils 1, B4000 Liège, Belgium Abstract This article shows the influence of a plane strain test specimen geometry on the measurable strain field and the influence of free edge effects over the stress computation. The experimental strain field distribution is measured over the whole deformable zone of a plane strain test specimen by an optical strain gauge. The chosen material is the DC06 IF steel of 0.8 mm thickness. The stress field is computed for several geometries at different strain levels by a Finite Element (FE) commercial code (Samcef ). The results show that the stress field is sensitive to the specimen's geometry and also to the tested material (strain field behavior is independent of material) and, based on results, an optimal specimen geometry is proposed in order to minimized the stress computation error. Keywords: Material characterization, mechanical tests, stress  strain field homogeneity. Introduction Industrial requirements for lighter components and structures have motivated the study of material behavior in order to save manufacturing and transportation energy. Different metal forming processes such as deep drawing, bending or stamping are required to manufacture automotive parts or beverage cans. The finite element method (FEM) is quite successful to simulate those metal forming processes, but accuracy depends both on the constitutive laws used and their material parameters identification. Constitutive models for sheet metal forming at room temperature include a yield surface defined by a yield criterion, a normality rule and a hardening law (yield surface evolution). Accurate phenomenological yield criteria are defined by material parameters that must be identified by several mechanical tests such as uniaxial tensile test, equibiaxial test, biaxial test, plane strain test and simple shear test. The goal of this work is to define a plane strain test specimen geometry in which the stress and the strain tensor fields have a quasihomogeneous behavior. A homogeneous behavior of those tensor fields allows the computation of the stress state directly from the force and deformation data and simplifies the parameters identification routines. The stress  strain state of the plane strain test and the experimental set up is described in next section. A strategy using FEM to study the stress field homogeneity is proposed in section 2. The results are discussed in section 3 and finally some conclusions are established and some perspectives proposed. Regarding notation, lowercase boldface Latin letters are used for vectors and uppercase boldface letters (Latin or Greek) to define second order tensor. The tensor product is defined by Description of the Plane Strain Test The plane strain test reproduces a particular case of the plane stress state in which one of the principal strain values and the shear components equal zero. This test is widely used in material characterization (yield surface and work hardening) and to obtain forming limits diagrams.
2 Mechanical Conditions Fig. 1 sketches the axis over a laminated sheet. The material axes defined by the rolling direction (RD), the transversal direction (TD) and the normal direction (ND) are coincident with the X 1, X 2 and X 3 axes. Assuming a plane stress state, the second order Cauchy stress tensor can be defined as follows: Figure 1: Rolled sheet axis definition, α defines the angle with respect to the RD. To represent the stress state for any angle a the following transformation linking a state defined in the x 1, x 2 and x 3 axes with the X 1, X 2 and X 3 is used: where R is a proper orthogonal second order tensor (i.e. R T R = RR T = I and det R = 1) defined by Then, the general expression for the plane stress state is defined as follows: The principal stretches of the sheet are represented by λ i (i = 1, 2, 3) in the second order stretch tensor U: The logarithmic strain is defined in terms of the principal stretches as: For the plane strain case λ 2 = 1, then ε 2 = 0. Assuming volume conservation, i.e., λ 1 λ 2 λ 3 = 1 (or ε 1 + ε 2 + ε 3 = 0), the logarithmic strain tensor components are related by ε 1 = ε 3.
3 In plasticity, the plastic strain rate tensor is related to the Cauchy stress tensor by the normality rule: where is the plastic multiplier and is the plastic potential function represented, in this work, by the Hill 1948 orthotropic yield criterion [1]: H, G, F, N, M, L are material parameters and k(p) describes the yield surface size evolution (isotropic hardening) in terms of the equivalent plastic strain. Using the condition ε 2 = 0 one can assume that: which allows the representation of one component of the Cauchy stress tensor in terms of the other (Eq. 10). This has particular significance when the stress data is used to identify yield function material parameters (e.g. when using the "plastic contours method" [2,3]) since most of the testing machines do not count with a proper device to measure the stress component in perpendicular direction with respect to the applied load. Eq. 10 can be seen as a generalization of the isotropic case when k a = 0,5. The relation shown in Eq. 10 can be obtained for other yield criteria as it is shown in [4]. Experimental set up Fig. 2a shows the biaxial testing machine built at the ArGEnCO Laboratory at the University of Liege [5]. The arrows in the figure show the machine movement axes. The motion is generated by two hydraulic pistons, which can be controlled in displacement or force simultaneously or independently. These motions enable us to perform simple shear and plane strain tests. Fig. 2b shows a detail of the specimen's measurable zone clamped by hydraulics grips. The specimen geometry designed for the biaxial testing machine is shown in Fig. 3a where the dotted area is the measurable zone. The deformation is imposed by the pistons (vertical for the plane strain test and horizontal for the simple shear test) of the biaxial testing machine. The strain field can be measured in the whole deformation zone (due to an optical strain gauge), and the average stress σ 11 is computed form the load cell data and the actual area as it is shown in Fig. 3b. This assumption is only valid if the stress field is homogeneous. The component σ 22 of the stress tensor cannot be measured with this mechanical configuration.
4 Figure 2: Biaxial testing machine designed at the ArGEnCO Laboratory, University of Liege. Figure 3: (a) Specimen geometry and deformation area, (b) Sketch of the stress distribution. Fig. 4 shows the experimental strain field distribution at the centerline level (Fig. 3b) for the logarithmic strain tensor components ε 11 and ε 22. The test is done over a DC06 IF steel of 0.8mm thickness (anyways, the strain distribution is independent of the material). The following conclusions can be drawn from these results: the strain tensor is homogeneous over the deformation area except at the free edges, the homogeneity depends on the amount of the imposed deformation (ε 11 ), the strain component ε 22 is negligible in the homogeneous zone of the deformation area and, by volume conservation, the condition ε 1 = ε 3 is valid over the homogeneous zone of the deformation area. These conclusions are valid for the specimen geometry of Fig. 4a, i.e., when h/b=10. The influence of deformation area geometry, the imposed strain level and the material over the stress field is studied in what follows by a FE simulation of the plane strain test.
5 Figure 4: (a) ε 11 strain distribution over the specimen centerline, (b) ε 22 strain distribution over the specimen centerline. Figure 5: Stress field in the loading direction for ε 11 = 20%, h/b=20 and thickness t=1.5mm.
6 Plane Strain Test FE Simulation The FE simulation of the test is used to study the stress field distribution over the deformable zone of the specimen. By studying the influence of the edge effect over several geometries, the obtained results help to define a criterion to define whether a stress field can be consider (quasi)homogeneous or heterogeneous. Simulation Parameters The simulation parameters appear in Table 1 and only the deformation area is simulated (sliding of the specimen inside the grips is neglected), the used mesh appears in Fig. 5. To study the influence of the material in the stress field, the results obtained out of two materials are compared. Material 1 corresponds to the IF steel DC06 characterized in [3,5], Material 2 is a Active material that has the same initial yield locus as Material 1, but a different hardening behavior (hardening stagnates at 10% of deformation). The initial yield locus material parameters for the Hill 1948 criterion (Eq. 8) are in Table 2 and Table 3 contains the hardening parameters. The elastic modulus is E = [MPa] and Poisson's coefficient v=0.3. Table 1: Finite element strategy. Code Element Type Finite Element Simulation Data Integration Points 8 Number of Elements Constitutive Law Samcef v1 1.1 (Samtech) Brick 5400 (3 thickness layers) Elastoplastic Hill 1948 coupled with isotropic hardening Table 2: Initial yield surface material parameters for Hill 1948 criterion. DC06 0.8mm Material Parameters for Hill 1948 criterion H F G N M L [MPa] Table 3: Hardening laws material parameters. Hardening Law Material Parameters for Hardening Laws Material Parameters Material 1 K [MPa] ε 0 n (DC06 0.8mm) k(p)=k(ε 0 +p) n Material 2 k(p) = σ y + R SAT [1exp(C R p)] σ y [MPa] R SAT [MPa] C R Comparing Variables The average stress is defined by Eq. 11, here V i represents the volume of the element, V total the total volume of the deformable area and σ i is the stress value of the element (in the loading direction). This stress computation is impossible to obtain experimentally. A second stress definition is given by Eq. 12. F is the load measured by the load cell and A CL is the cross section area computed at the centerline of the specimen's deformation area. In this case, the stress value can be obtained
7 experimentally but it involves expensive equipment and it is time consuming. A third definition is presented in Eq. 13. F is the load measured by the load cell and A CP is the cross section area computed with the information obtained at the center point of the specimen's deformation area. Assuming volume conservation in plasticity, this cross section area can be obtained from Eq. 14, where A 0 is the initial cross section area of the specimen and ε CP 11 is the strain measured in the load direction at the center point of the deformation area. Then, in order to define a homogeneity criterion, the stress values obtained from Eq. 12 and 13 are compared with the one given for Eq. 11 for a quasihomogeneous, arbitrary chosen, stress distribution. This reference stress is obtained from a geometrical ratio of h/b=20 (a higher ratio would not be economically viable) and t=1.5mm since the absolute relative error between σ global (or σ true ) and σ ave is not greater than 0.5% for an imposed strain of 20% for Material 1 (see Fig. 5) and 10% for Material 2. Results Fig. 6 shows the error at different strain levels for different specimen's geometries. It is clear that increasing the ratio h/b, the error between the average stress (taken as a reference value) and the global and true stress diminish. The influence of the strain level does not seem to have a large influence on the error evolution. The error obtained by using the true stress definition is less than 0.2% in the most adverse case (h/b=5) when comparing with the error given by the global stress definition, this means that for a ratio higher than h/b=10 the actual area can be obtained from measures taken at the center of the specimen (Eq. 14), saving important data processing time. Fig. 7 shows that the stress error depends on the material (unlike the strain fields), hence it makes impossible to compute a general correction factor. Fig. 8 shows that homogeneity also depends (slightly) on the specimen's thickness.
8 Figure 6: Stress error in terms of h/b for Material 1, (a) for σ global, (b) for σ true.
9 Figure 7: Differences of the stress error depending on the material, (a) for σ giobai, (b) for σ true.
10 Figure 8: Influence of the thickness specimen in the error.
11 Figure 9: Modifications at the free edge levels of the specimen.
12 Conclusions and Perspectives The geometrical ratio h/b=10 in the measurable zone of the specimen geometry seems to be the most performing since the stress error is less than 1% for the two materials. It also ensures that the strain in the sense perpendicular to the impose deformation ε 22 remains negligible during the deformation process. The actual area can be measured from the center point data. The thickness variation does not seem to contribute significantly to the stress error. Even if the final stress error could be quantified, this has not practical interest since the stress field is dependent on the material; hence it is impossible to define a general correction factor. From this work another criterion of homogeneity can be proposed in order to neglect the component ε 22 in the strain tensor: the strain average taken over an 80% of central part of the deformation area must by much lower than the one measure at the free edges (as observed in Fig. 4b). In this case, it is necessary to compute the whole strain field. In future, the specimen geometry will be slightly modified at the free edge level (Fig. 9) in order to study the failure position which occurs near the free edges, where strain and stress concentrations are higher as it is shown respectively in Fig. 4 and Fig. 5. Acknowledgement As Research Director, AnneMarie Habraken would like to thank the National Found for Scientific Research (FNRS, Belgium) for its support. References [1] R. Hill: The Mathematical Theory of Plasticity (The Oxford Eng Sciences Series, 1950). [2] T. Kuwabara, A. Van Beal, E. Iizuka: Acta Materialia Vol. 50 (2002), pp [3] P. Flores, P. Moureaux, A.M. Habraken: Material Identification using a Biaxial Test Machine (Trans Tech Publications, Switzerland 2005). [4] P. Flores: Development of Experimental Equipment and Identification Procedures for Sheet Metal Constitutive Laws (PhD Thesis, University of Liege  Belgium, 2005). [5] P. Flores, E. Rondia, A.M. Habraken: International Journal of Forming Processes, Special Issue (2005) pp
Numerical simulation of sheet metal forming processes using a new yield criterion
Key Engineering Materials Vol. 344 (007) pp. 833840 online at http://www.scientific.net (007) Trans Tech Publications, Switzerland Numerical simulation of sheet metal forming processes using a new yield
More informationCOMPARISON OF THE TESTS CHOSEN FOR MATERIAL PARAMETER IDENTIFICATION TO PREDICT SINGLE POINT INCREMENTAL FORMING FORCES
International Deep Drawing Research Group IDDRG 28 International Conference 1618 June 28, Olofström, Sweden COMPARISON OF THE TESTS CHOSEN FOR MATERIAL PARAMETER IDENTIFICATION TO PREDICT SINGLE POINT
More informationSTRESS UPDATE ALGORITHM FOR NONASSOCIATED FLOW METAL PLASTICITY
STRESS UPDATE ALGORITHM FOR NONASSOCIATED FLOW METAL PLASTICITY Mohsen Safaei 1, a, Wim De Waele 1,b 1 Laboratorium Soete, Department of Mechanical Construction and Production, Ghent University, Technologiepark
More informationStudy of Axes Rotation during Simple Shear Tests on Aluminum Sheets
Study of xes Rotation during Simple Shear ests on luminum Sheets L. Duchêne 1, B. Diouf 1,. Lelotte 1, P. Flores 1, S. Bouvier 2,.M. Habraken 1 1. rgenco Dept., University of Liège, Chemin des Chevreuils
More informationSPRINGBACK PREDICTION FOR STAMPINGS FROM THE THIN STAINLESS SHEETS
SPRINGBACK PREDICTION FOR STAMPINGS FROM THE THIN STAINLESS SHEETS PAVEL SOLFRONK, JIRI SOBOTKA, MICHAELA KOLNEROVA, LUKAS ZUZANEK Technical University of Liberec Faculty of Mechanical Engineering Department
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationThe objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties.
Objective: The objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties. Introduction: Mechanical testing plays an important role
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationBack Analysis and optimization methods with LAGAMINE
Back Analysis and optimization methods with LAGAMINE Séverine Levasseur Chantal Bouffioux Université de Liège First International Workshop on the Finite Element Code LAGAMINE LAGASHOP 2013, Liège, 9 12
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationLecture #8: Ductile Fracture (Theory & Experiments)
Lecture #8: Ductile Fracture (Theory & Experiments) by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing 2015 1 1 1 Ductile
More informationIDENTIFICATION OF SHEET METAL PLASTIC ANISOTROPY, AND OPTIMIZATION OF INITIAL BLANK SHAPE IN DEEP DRAWING
THE ANNALS OF DUNĂREA DE JOS UNIVERSITY OF GALAŢI FASCICLE V, TECHNOLOGIES IN MACHINE BUILDING, ISSN  66, 9 IDENTIFICATION OF SHEET METAL PLASTIC ANISOTROPY, AND OPTIMIZATION OF INITIAL BLANK SHAPE IN
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationMaterial parameter identification for the numerical simulation of deepdrawing drawing of aluminium alloys
Material parameter identification for the numerical simulation of deepdrawing drawing of aluminium alloys B.M. Chaparro, J.M. Antunes, A.J. Baptista, D.M. Rodrigues,, J.V. Fernandes, L.F. Menezes M2D'26
More informationShock enhancement of cellular structures under impact loading: Part II Analysis
Shock enhancement of cellular structures under impact loading: Part II Analysis S. Pattofatto, 1 I. Elnasri, 1 H. Zhao, 1* H. Tsitsiris 1 F. Hild 1 and Y. Girard 2 1 Laboratoire de Mécanique et Technologie
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationA ratedependent HosfordCoulomb model for predicting ductile fracture at high strain rates
EPJ Web of Conferences 94, 01080 (2015) DOI: 10.1051/epjconf/20159401080 c Owned by the authors, published by EDP Sciences, 2015 A ratedependent HosfordCoulomb model for predicting ductile fracture at
More informationTHE HYDRAULIC BULGE TEST AND ITS IMPORTANCE FOR THE VEGTER YIELD CRITERION
THE HYDRAULIC BULGE TEST AND ITS IMPORTANCE FOR THE VEGTER YIELD CRITERION Jiří SOBOTKA a, Pavel SOLFRONK a, Pavel DOUBEK a, Lukáš ZUZÁNEK a a TECHNICAL UNIVERSITY OF LIBEREC, Studentská, 461 17 Liberec
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationExperiment Two (2) Torsional testing of Circular Shafts
Experiment Two (2) Torsional testing of Circular Shafts Introduction: Torsion occurs when any shaft is subjected to a torque. This is true whether the shaft is rotating (such as drive shafts on engines,
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationCharacterizations of Aluminum Alloy Sheet Materials Numisheet 2005
Characterizations of Aluminum Alloy Sheet Materials Numisheet 25 John C. Brem, Frederic Barlat, Robert E. Dick, and JeongWhan Yoon Alcoa Technical Center, PA, 15691, USA Abstract. This report reproduces
More informationEvaluation of inplane orthotropic elastic constants of paper and paperboard
Evaluation of inplane orthotropic elastic constants of paper and paperboard T. Yokoyama and K. Nakai Department of Mechanical Engineering, Okayama University of Science  Ridaicho, Okayama 75, Japan
More informationThis article appeared in a journal published by Elsevier. The attached copy is furnished to the author for internal noncommercial research and
This article appeared in a journal published by Elsevier. The attached copy is furnished to the author for internal noncommercial research and education use, including for instruction at the authors institution
More informationPlasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur
Plasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 9 Table of Contents 1. Plasticity:... 3 1.1 Plastic Deformation,
More informationNonlinear FE Analysis of Reinforced Concrete Structures Using a TrescaType Yield Surface
Transaction A: Civil Engineering Vol. 16, No. 6, pp. 512{519 c Sharif University of Technology, December 2009 Research Note Nonlinear FE Analysis of Reinforced Concrete Structures Using a TrescaType Yield
More informationStructural behaviour of traditional mortiseandtenon timber joints
Structural behaviour of traditional mortiseandtenon timber joints Artur O. Feio 1, Paulo B. Lourenço 2 and José S. Machado 3 1 CCR Construtora S.A., Portugal University Lusíada, Portugal 2 University
More informationBending Load & Calibration Module
Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationIDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE Hugo Sol, hugos@vub.ac.be Massimo Bottiglieri, Massimo.Bottiglieri@vub.ac.be Department Mechanics of Materials
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM BEHAVIOR UNDER THE EFFECT OF EXTERNAL SOLICITATIONS
Third International Conference on Energy, Materials, Applied Energetics and Pollution. ICEMAEP016, October 3031, 016, Constantine,Algeria. ANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationStrain Measurement. Prof. Yu Qiao. Department of Structural Engineering, UCSD. Strain Measurement
Strain Measurement Prof. Yu Qiao Department of Structural Engineering, UCSD Strain Measurement The design of loadcarrying components for machines and structures requires information about the distribution
More informationOptimum Height of Plate Stiffener under Pressure Effect
The st Regional Conference of Eng. Sci. NUCEJ Spatial ISSUE vol., No.3, 8 pp 459468 Optimum Height of Plate Stiffener under Pressure Effect Mazin Victor Yousif M.Sc Production Engineering University of
More informationA novel approach to predict the growth rate of short cracks under multiaxial loadings
A novel approach to predict the growth rate of short cracks under multiaxial loadings F. Brugier 1&2, S. Pommier 1, R. de Moura Pinho 2, C. Mary 2 and D. Soria 2 1 LMTCachan, ENS Cachan / CNRS / UPMC
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationConstitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationLecture #6: 3D Rateindependent Plasticity (cont.) Pressuredependent plasticity
Lecture #6: 3D Rateindependent Plasticity (cont.) Pressuredependent plasticity by Borja Erice and Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling
More informationINCREASING RUPTURE PREDICTABILITY FOR ALUMINUM
1 INCREASING RUPTURE PREDICTABILITY FOR ALUMINUM Influence of anisotropy Daniel Riemensperger, Adam Opel AG Paul Du Bois, PDB 2 www.opel.com CONTENT Introduction/motivation Isotropic & anisotropic material
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationComputational Inelasticity FHLN05. Assignment A nonlinear elastoplastic problem
Computational Inelasticity FHLN05 Assignment 2018 A nonlinear elastoplastic problem General instructions A written report should be submitted to the Division of Solid Mechanics no later than November
More informationConstitutive model for quasistatic deformation of metallic sandwich cores
INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING Int. J. Numer. Meth. Engng 2004; 61:2205 2238 Published online 18 October 2004 in Wiley InterScience (www.interscience.wiley.com). DOI: 10.1002/nme.1142
More informationEffective stress method to be used in beam finite elements to take local instabilities into account
Effective stress method to be used in beam finite elements to take local instabilities into account JEANMARC FRANSSEN, BAPTISTE COWEZ and THOMAS GERNAY ArgencoDepartment University of Liège Chemin des
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationStructural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More informationStresses Analysis of Petroleum Pipe Finite Element under Internal Pressure
ISSN : 4896, Vol. 6, Issue 8, ( Part 4 August 06, pp.338 RESEARCH ARTICLE Stresses Analysis of Petroleum Pipe Finite Element under Internal Pressure Dr.Ragbe.M.Abdusslam Eng. Khaled.S.Bagar ABSTRACT
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationAnalytical and experimental evaluation of the stressstrain curves of sheet metals by hydraulic bulge tests
Analytical and experimental evaluation of the stressstrain curves of sheet metals by hydraulic bulge tests Lucian LĂZĂRESCU 1, a, DanSorin COMŞA 1,b and Dorel BANABIC 1,c 1 Technical University of ClujNapoca,
More informationEffective stress method to be used in beam finite elements to take local instabilities into account
Effective stress method to be used in beam finite elements to take local instabilities into account JEANMARC FRANSSEN, BAPTISTE COWEZ ans THOMAS GERNAY Argenco Department University of Liège Chemin des
More informationHardened Concrete. Lecture No. 16
Hardened Concrete Lecture No. 16 Fatigue strength of concrete Modulus of elasticity, Creep Shrinkage of concrete StressStrain Plot of Concrete At stress below 30% of ultimate strength, the transition
More informationOptimization of blank dimensions to reduce springback in the flexforming process
Journal of Materials Processing Technology 146 (2004) 28 34 Optimization of blank dimensions to reduce springback in the flexforming process Hariharasudhan Palaniswamy, Gracious Ngaile, Taylan Altan ERC
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationThe effect of restraints type on the generated stresses in gantry crane beam
The effect of restraints type on the generated stresses in gantry crane beam Leszek Sowa 1,*, Wiesława Piekarska 1, Tomasz Skrzypczak 1, Paweł Kwiatoń 1 1 Czestochowa University of Technology, Institute
More informationResearch Article Process of Identifying Stress Fields from Strain Fields in the Specimen with a Hole
ISRN Materials Science Volume 213, Article ID 53669, 8 pages http://dx.doi.org/1.1155/213/53669 Research Article Process of Identifying Stress Fields from Strain Fields in the Specimen with a Hole Michaela
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationScienceDirect. Bauschinger effect during unloading of coldrolled copper alloy sheet and its influence on springback deformation after Ubending
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 81 (2014 ) 969 974 11th International Conference on Technology of Plasticity, ICTP 2014, 1924 October 2014, Nagoya Congress
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More information3D Finite Element Analysis of Instrumented Indentation of Transversely Isotropic Materials
3D Finite Element Analysis of Instrumented Indentation of Transversely Isotropic Materials Abstract: Talapady S. Bhat and T. A. Venkatesh Department of Material Science and Engineering Stony Brook University,
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationINVERSE METHOD FOR FLOW STRESS PARAMETERS IDENTIFICATION OF TUBE BULGE HYDROFORMING CONSIDERING ANISOTROPY
7 th EUROMECH Solid Mechanics Conference J. Ambrósio et.al. (eds.) Lisbon, Portugal, September 711, 2009 INVERSE METHOD FOR FLOW STRESS PARAMETERS IDENTIFICATION OF TUBE BULGE HYDROFORMING CONSIDERING
More informationLecture 8 Viscoelasticity and Deformation
Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, µ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force to the strain in the direction of the applied force. For uniaxial
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationThe Rotating Inhomogeneous Elastic Cylinders of. VariableThickness and Density
Applied Mathematics & Information Sciences 23 2008, 237 257 An International Journal c 2008 Dixie W Publishing Corporation, U. S. A. The Rotating Inhomogeneous Elastic Cylinders of VariableThickness and
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationAnisotropic plasticity, anisotropic failure and their application to the simulation of aluminium extrusions under crash loads
Anisotropic plasticity, anisotropic failure and their application to the simulation of aluminium extrusions under crash loads Paul Du Bois, Consulting engineer Oasys LSDYNA Users Meeting 28th January
More informationHIGHLY ADAPTABLE RUBBER ISOLATION SYSTEMS
th World Conference on Earthquake Engineering Vancouver, B.C., Canada August 6, 24 Paper No. 746 HIGHLY ADAPTABLE RUBBER ISOLATION SYSTEMS Luis DORFMANN, Maria Gabriella CASTELLANO 2, Stefan L. BURTSCHER,
More informationAbstract. 1 Introduction
Contact analysis for the modelling of anchors in concrete structures H. Walter*, L. Baillet** & M. Brunet* *Laboratoire de Mecanique des Solides **Laboratoire de Mecanique des ContactsCNRS UMR 5514 Institut
More informationCHAPTER 7 FINITE ELEMENT ANALYSIS OF DEEP GROOVE BALL BEARING
113 CHAPTER 7 FINITE ELEMENT ANALYSIS OF DEEP GROOVE BALL BEARING 7. 1 INTRODUCTION Finite element computational methodology for rolling contact analysis of the bearing was proposed and it has several
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationA study of forming pressure in the tubehydroforming process
Journal of Materials Processing Technology 192 19 (2007) 404 409 A study of forming pressure in the tubehydroforming process FuhKuo Chen, ShaoJun Wang, RayHau Lin Department of Mechanical Engineering,
More informationOn the Numerical Modelling of Orthotropic Large Strain Elastoplasticity
63 Advances in 63 On the Numerical Modelling of Orthotropic Large Strain Elastoplasticity I. Karsaj, C. Sansour and J. Soric Summary A constitutive model for orthotropic yield function at large strain
More informationInverse identification of plastic material behavior using. multiscale virtual experiments
Inverse identification of plastic material behavior using multiscale virtual experiments Debruyne 1 D., Coppieters 1 S., Wang 1 Y., Eyckens 2 P., Kuwabara 3 T., Van Bael 2 A. and Van Houtte 2 P. 1 Department
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationCHAPTER 5. Beam Theory
CHPTER 5. Beam Theory SangJoon Shin School of Mechanical and erospace Engineering Seoul National University ctive eroelasticity and Rotorcraft Lab. 5. The EulerBernoulli assumptions One of its dimensions
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationModelling and numerical simulation of the wrinkling evolution for thermomechanical loading cases
Modelling and numerical simulation of the wrinkling evolution for thermomechanical loading cases Georg Haasemann Conrad Kloß 1 AIMCAL Conference 2016 MOTIVATION Wrinkles in web handling system Loss of
More information